DETAILS OF CORROSION AND CORROSION
DATE: NOVEMBER/DECEMBER 2012
STUDENT NUMBER: 201214830
1. INTRODUCTION ON CORROSION
Environment plays a role in corrosion formation thus Corrosion can be defined as the
dilapidation or degradation of a material due to a reaction with its environment.
Degradation or dilapidation implies weakening of physical properties of the material.
This can be a weakening of the material due to a loss of cross-sectional area, it can be
the shattering of a metal due to hydrogen embrittlement, or it can be the cracking of a
polymer due to sunlight exposure. Corrosion not only occurs in metals but it is a
broad concept which applies to all materials, thus the term material in this context
refer to metals, polymers, ceramics or composites of two or more materials with
2. METALLIC CORROSION: WHY METALS CORRODE
As described in part 1 of this report environment plays a role towards material
corrosion, metals are no exception. Chemically unstable environments which metals
are exposed to results in metals corroding. Most metals are unstable in nature, in most
case metals which are processed minerals this does not include precious metals such
as gold, platinum, silver etc. Precious metals are thermodynamically stable at room
temperature and are not susceptible to corrosion. The theory that has been used to
describe the mechanism of corrosion is the theory of Electrochemistry. This theory
addresses the oxidation-reduction reactions that take place when a metal corrodes and
explains it from atomic level. In other words for a metal to corrode the must be some
oxidation and reduction reactions taking place and this normally happens when metals
3. FORMS OF CORROSION
This is also called general corrosion. The surface effect produced by most direct
chemical attacks is a uniform etching of the metal. Some schools of thoughts
define it as a type of corrosion where by the thickness is reduced equally or the
type of corrosion which causes the metal to corrode at the same amount ( see
figure 1). On a polished surface, this type of corrosion is first seen as a general
dulling of the surface and, if allowed to continue, the surface becomes rough and
possibly frosted in appearance. The discoloration or general dulling of metal
created by its exposure to elevated temperatures is not to be considered as uniform
etch corrosion. The use of chemical-resistant protective coatings or more resistant
materials will control these problems. While this is the most common form of
corrosion, it is generally of little engineering significance, because structures will
normally become unsightly and attract maintenance long before they become
Figure 1: Uniform reduction of thickness
The figure below show a typical uniform corrosion:
Galvanic corrosion is an electrochemical action of two dissimilar metals in the
presence of an electrolyte and an electron conductive path. It occurs when
dissimilar metals are in contact.It is recognizable by the presence of a build-up of
corrosion at the joint between the dissimilar metals. For example, when aluminum
alloys or magnesium alloys are in contact with steel (carbon steel or stainlesssteel), galvanic corrosion can occur and accelerate the corrosion of the aluminum
or magnesium. The figure below shows a pictorial description of galvanic
3.3. PITTING CORROSION
Inactive metals, such as stainless steel, resist corrosive media and can perform
well over long periods of time. However, if corrosion does occur, it forms at
random in pits. Pitting is most likely to occur in the presence of chloride ions,
combined with such depolarizers as oxygen or oxidizing salts. Methods that can
be used to control pitting include maintaining clean surfaces, application of a
protective coating, and use of inhibitors or cathodic protection for immersion
service. Molybdenum additions to stainless steel are intended to reduce pitting
corrosion. The figure below shows pitting corrosion:
The rust bubbles on the cast iron above indicate that pitting is occurring.
Researchers have found that the environment inside the rust bubbles is almost
always higher in chlorides and lower in pH (more acidic) than the overall external
environment. This leads to concentrated attack inside the pits. Figure below shows
Crevice or contact corrosion is the corrosion produced at the region of contact of
metals with metals or metals with non-metals. It may occur at washers, under
barnacles, at sand grains, under applied protective films, and at pockets formed by
threaded joints. Whether or not stainless steels are free of pit nuclei, they are
always susceptible to this kind of corrosion because a nucleus is not necessary.
Cleanliness, the proper use of sealants, and protective coatings are effective means
of controlling this problem. Molybdenum-containing grades of stainless steel have
increased crevice corrosion resistance.
The crevice corrosion shown below happened when an aerospace alloy (titanium 6 aluminum - 4 vanadium) was used instead of a more corrosion-resistant grade of
titanium. Special alloying additions are added to titanium to make alloys which
are crevice corrosion resistant even at elevated temperature.
Inter-granular corrosion is an attack on or adjacent to the grain boundaries of a
metal or alloy. A highly magnified cross section of most commercial alloys will
show its granular structure. This structure consists of quantities of individual
grains, and each of these tiny grains has a clearly defined boundary that
chemically differs from the metal within the grain centre. Heat treatment of
stainless steels and aluminum alloys accentuates this problem.
The picture below shows a stainless steel which corroded in the heat affected zone
a short distance from the weld. This is typical of inter-granular corrosion in
austenitic stainless steels. This corrosion can be eliminated by using stabilized
stainless steels by using low-carbon stainless grades.
Exfoliation is a form of inter-granular corrosion. It manifests itself by lifting up the
surface grains of a metal by the force of expanding corrosion products occurring at the
grain boundaries just below the surface. It is visible evidence of inter-granular
corrosion and most often seen on extruded sections where grain thickness is less than
in rolled forms. This form of corrosion is common on aluminum, and it may occur on
The picture above shows exfoliation corrosion in aluminium.
3.6.SCC – STRESS CRACK CORROSION
Stress corrosion cracking (SCC) is caused by the simultaneous effects of tensile
stress and a specific corrosive environment. Stresses may be due to applied loads,
residual stresses from the manufacturing process, or a combination of both.
Cross sections of SCC frequently show branched cracks. This river branching
pattern is unique to SCC and is used in failure analysis to identify when this form
of corrosion has occurred. The picture below shows that:
The photo below shows SCC of an insulated stainless-steel condensate line. Water
wetted the insulation and caused chlorides to leach from the insulation onto the
hot metal surface. This is a common problem on steam and condensate lines.
Control is by maintaining the jackets around the lines so that moisture doesn't
enter the insulation or is quickly drained off.
The next two photos show intergranular SCC of an aluminum aerospace part. The
intergranular nature of the corrosion can be seen in the scanning electron
microscope image on the left and in the microscopic cross section on the right.
The arrows indicate the primary crack shown in both pictures. Note that secondary
cracks are also apparent. These secondary cracks are common in stress corrosion
The rapid corrosion that occurs at the interface between contacting, highly loaded
metal surfaces when subjected to slight vibratory motions is known as fretting
The figure below shows fretting corrosion of a fence post and wires which swing
in the wind and wear against the post. Both the fence post and the connecting
wires are experiencing fretting corrosion.
This type of corrosion is most common in bearing surfaces in machinery, such as
connecting rods, splined shafts, and bearing supports, and often causes a fatigue
failure. It can occur in structural members such as trusses where highly loaded
bolts are used and some relative motion occurs between the bolted members.
Fretting corrosion is greatly retarded when the contacting surfaces can be well
lubricated as in machinery-bearing surfaces so as to exclude direct contact with
The bearing race above is a classic example of fretting corrosion. This is greatly
retarded when the contacting surfaces can be well lubricated as in machinerybearing surfaces so as to exclude direct contact with air.
Microbial corrosion (also called microbiologically-influenced corrosion or MIC)
is corrosion that is caused by the presence and activities of microbes. This
corrosion can take many forms and can be controlled by biocides or by
conventional corrosion control methods. There are a number of mechanisms
associated with this form of corrosion, and detailed explanations are available at
the web sites listed at the bottom of this section. Most MIC takes the form of pits
that form underneath colonies of living organic matter and mineral and biodeposits. This biofilm creates a protective environment where conditions can
become quite corrosive and corrosion is accelerated.
The picture below shows a biofilm on a metallic condenser surface. Thus the
corrosive conditions corrosive chemicals to collect within and under the films.
Thus the corrosive conditions under a biofilm can be very aggressive, even in
locations where the bulk environment is noncorrosive.
Other pictures showing microbial corrosion are shown below:
4. CORROSION CONTROL
Correct material selection for certain applications
David E.J. & ames D.R. (1997). Corrosion Science and Technology. CRC Press:
Ewald H. (1996). Microbially influenced corrosion of materials:scientific and
engineering aspects. Springer-Verlag:Detroit
Shreir L.L. (1976). Corrosion: Corrosion control. Newnes-Butterworths: Detroit